- Nano Express
- Open Access
Nanoscale anisotropic plastic deformation in single crystal GaN
© Huang et al; licensee Springer. 2012
- Received: 8 October 2011
- Accepted: 22 February 2012
- Published: 22 February 2012
Elasto-plastic mechanical deformation behaviors of c-plane (0001) and nonpolar GaN single crystals are studied using nanoindentation, cathodoluminescence, and transmission electron microscopy. Nanoindentation tests show that c-plane GaN is less susceptible to plastic deformation and has higher hardness and Young's modulus than the nonpolar GaN. Cathodoluminescence and transmission electron microscopy characterizations of indent-induced plastic deformation reveal that there are two primary slip systems for the c-plane GaN, while there is only one most favorable slip system for the nonplane GaN. We suggest that the anisotropic elasto-plastic mechanical properties of GaN are relative to its anisotropic plastic deformation behavior.
PACS: 62.20.fq; 81.05.Ea; 61.72.Lk.
- hydride vapor phase epitaxy
- transmission electron microscopy.
GaN-related III-nitride materials are attracting increasing attention for a wide range of device applications, such as light-emitting diodes , blue laser devices , and high electron mobility transistor . Besides, GaN also exhibits attractive mechanical properties for potential device manufacture such as making microelectromechanical systems and making surface acoustic wave device [4, 5]. Therefore, there is an increasingly growing interest in the elasto-plastic mechanical behaviors of GaN material [6–16].
The previous investigations in the elasto-plastic mechanical behaviors of GaN were mainly carried out on a c-plane GaN. The only few works performed on nonpolar ((11-20) and (10-10) planes) GaN epitaxial layers, however, were largely affected by the substrate or the growth induced stacking faults [6–16]. Moreover, despite it is well known that GaN crystallizes in the wurtzite structure is characterized by a high anisotropy, a study on anisotropic elasto-plastic mechanical behaviors of GaN is still lacking.
This work attempts to present nanoindentation experiments performed on the three principal surfaces, (0001), (11-20), and (10-10), of GaN single crystals. Furthermore, the underlying activated slip systems which govern the plastic deformation of GaN are identified by cathodoluminescence (CL) and transmission electron microscopy. Finally, a comparison between the c-plane and nonpolar GaN in mechanical properties and plastic deformation is presented.
The samples under investigations were grown by hydride vapor phase epitaxy in homemade reactor. The c-plane GaN samples were obtained from a 1.5-mm thick free standing GaN wafer with dislocation density lower than 106 cm-2. Also, the a-plane and m-plane samples were obtained from a 1.5-mm thick free standing GaN wafer by cleaving along the (11-20) and (10-10) planes, respectively. The crystal orientations were identified by X-ray diffraction. The mechanical properties of GaN crystals were conducted with a nanoindentation system (Nano indenter G200, Agilent Technologies Inc., Santa Clara, CA, USA). The analytical method developed by Oliver and Pharr  was adopted to determine the hardness (H) and Young's modulus (E) of the GaN crystals from indentations with a maximum penetration depth of 500 nm. Scanning electron microscopy (Quanta 400 FEG, FEI Company, Hillsboro, OR, USA) and its attached cathodoluminescence (MonoCL3+) (SEM-CL) were combined to characterize the indentation-induced plastic deformation at room temperature. The cross-sectional transmission electron microscopy (XTEM) samples were prepared from the indents by means of a dual-beam focused ion beam (Nova 220) station with Ga ions. A FEI Tecnai G2 F20 S-Twin TEM operated at an accelerating voltage of 200 kV was used to study the microstructures of obtained XTEM samples.
Indenter tip, contact plane, Young's modulus (E), and hardness (H) of GaN single crystal
333.61 ± 2.70
19.04 ± 0.23
330.56 ± 2.72
15.31 ± 0.20
329.74 ± 3.26
15.24 ± 0.21
317.34 ± 4.12
20.16 ± 0.48
308.26 ± 3.82
15.87 ± 0.41
306.96 ± 3.98
16.23 ± 0.44
Values were obtained from nanoindentation tests on GaN single crystal. The data from the indentation tests represent average data from at least 20 valid initial values. Also, the mean square error of each average data is given in the table. Values of E and H were calculated by Oliver and Pharr method  using load-depth curve of Figure 1.
In order to fully understand the deformation mechanism of c-plane GaN and nonpolar GaN under nanoindentation, the damages induced by conical tip were investigated by CL and XTEM (the damages induced by Berkovich tip is similar to but have less symmetry than those induced by conical tip).
To further elucidate the slip band of nanoindentation-induced deformation, an indent with maximum depth of 500 nm in c-plane GaN is investigated by XTEM. Figure 2b displayed a dark-field XTEM picture in the vicinity of the indented region. The picture displays a microstructure of the slip bands, characterized by features of aligned bright lines in the photograph. It can be seen clearly that the slip bands aligned parallel to the (0001) basal plane intersect the slip bands propagating along the (10-11) pyramidal plane. The two sets of slip bands suggest that during the indentation, the rapidly increasing dislocations can glide collectively along those planes. Moreover, selected area diffraction patterns of the highly damaged regions directly beneath the indenter showed no evidence of structural transformations to other phases of GaN. Therefore, the dislocations gliding along both the (0001) basal planes and the (10-11) pyramidal planes should be the primary mechanism of plastic deformation on the c-plane GaN during loading. The result is consistent with the previous reports [6, 8, 10–12].
To summarize, the anisotropic mechanical properties and deformation behavior based on high-quality GaN bulk material were presented in this paper. Nanoindentation tests reveal that nonpolar GaN has lower values than the c-plane GaN in both Young's modulus and hardness. Also, CL and XTEM measurements show that there are two primary dislocation slip planes ((0001) and (10-11) planes) for c-plane GaN, while there is only one most favorable dislocation slip plane ((0001) plane) for nonplane GaN during plastic deformation. We suggest that the anisotropic elasto-plastic mechanical properties of GaN are relative to its anisotropic plastic deformation behavior.
We thank the help from Suzhou Nanowin Science and Technology Co., Ltd. (NANOWIN) for the growth of samples. This work was partly supported by the National Natural Science Foundation of China (grant no. 51002179).
- Ponce FA, Bour DP: Nitride-based semiconductors for blue and green light-emitting devices. Nature 1997, 386: 351. 10.1038/386351a0View ArticleGoogle Scholar
- Nakamura S: The roles of structural imperfections in InGaN-based blue light-emitting diodes and laser diodes. Science 1998, 281: 956.View ArticleGoogle Scholar
- Ambacher O, Foutz B, Smart J, Shealy JR, Weimann NG, Chu K, Murphy M, Sierakowski AJ, Schaff WJ, Eastman LF, Dimitrov R, Mitchell A, Stutzmann M: Two dimensional electron gases induced by spontaneous and piezoelectric polarization in undoped and doped AlGaN/GaN heterostructures. J Appl Phys 2000, 87: 334. 10.1063/1.371866View ArticleGoogle Scholar
- Cimalla V, Pezoldt J, Ambacher O: Group III nitride and SiC based MEMS and NEMS: materials properties, technology and applications. J Phys D: Appl Phys 2007, 40: 6386. 10.1088/0022-3727/40/20/S19View ArticleGoogle Scholar
- Pedros J, Calle F, Cuerdo R, Grajal J, Bougrioua Z: Voltage tunable surface acoustic wave phase shifter on AlGaN/GaN. Appl Phys Lett 2010, 96: 123505. 10.1063/1.3353971View ArticleGoogle Scholar
- Bradby JE, Kucheyev SO, Williams JS, Wong-Leung J, Swain MV, Munroe P, Li G, Phillips MR: Indentation-induced damage in GaN epilayers. Appl Phys Lett 2002, 80: 383. 10.1063/1.1436280View ArticleGoogle Scholar
- Jahn U, Trampert A, Wagner T, Brandt O, Ploog KH: Indentation of GaN: a study of the optical activity and strain state of extended defects. Phys Stat Sol (a) 2002, 192: 79. 10.1002/1521-396X(200207)192:1<79::AID-PSSA79>3.0.CO;2-5View ArticleGoogle Scholar
- Chien CH, Jian SR, Wang CT, Juang JY, Huang JC, Lai YS: Cross-sectional transmission electron microscopy observations on the Berkovich indentation-induced deformation microstructures in GaN thin films. J Phys D: Appl Phys 2007, 40: 3985. 10.1088/0022-3727/40/13/011View ArticleGoogle Scholar
- Fujikane M, Leszczyski M, Nagao S, Nakayama T, Yamanaka S, Niihara K, Nowak R: Elastic-plastic transition during nanoindentation in bulk GaN crystal. J Alloys Compd 2008, 450: 405. 10.1016/j.jallcom.2006.10.121View ArticleGoogle Scholar
- Jian SR: Berkovich indentation-induced deformation behaviors of GaN thin films observed using cathodoluminescence and cross-sectional transmission electron microscopy. Appl Surf Sci 2008, 254: 6749. 10.1016/j.apsusc.2008.04.078View ArticleGoogle Scholar
- Jian SR: Mechanical deformation induced in Si and GaN under Berkovich nanoindentation. Nanoscale Res Lett 2008, 3: 6. 10.1007/s11671-007-9106-0View ArticleGoogle Scholar
- Jian SR, Juang JY, Lai YS: Cross-sectional transmission electron microscopy observations of structural damage in Al0.16Ga0.84N thin film under contact loading. J Appl Phys 2008, 103: 033503. 10.1063/1.2836939View ArticleGoogle Scholar
- Tsai CH, Jian SR, Juang JY: Berkovich nanoindentation and deformation mechanisms in GaN thin films. Appl Surf Sci 2008, 254: 1997. 10.1016/j.apsusc.2007.08.022View ArticleGoogle Scholar
- Wei TB, Hu Q, Duan RF, Wang JX, Zeng YP, Li JM, Yang Y, Liu YL: Mechanical deformation behavior of nonpolar GaN thick films by Berkovich nanoindentation. Nanoscale Res Lett 2009, 4: 753. 10.1007/s11671-009-9310-1View ArticleGoogle Scholar
- Lin MH, Wen HC, Huang CY, Jeng YR, Yau WH, Wu WF, Chou CP: Nanoindentation characterization of GaN epilayers on A-plane sapphire substrates. Appl Surf Sci 2010, 256: 3464. 10.1016/j.apsusc.2009.12.054View ArticleGoogle Scholar
- Fujikane M, Inoue A, Yokogawa T, Nagao S, Nowak R: Mechanical properties characterization of c-plane (0001) and m-plane (10–10) GaN by nanoindentation examination. Phys Status Solidi C 2010, 7: 1798. 10.1002/pssc.200983641View ArticleGoogle Scholar
- Oliver WC, Pharr GM: An improved technique for determining hardness and elastic-modulus using load and displacement sensing indentation experiments. J Mater Res 1992, 7: 1564. 10.1557/JMR.1992.1564View ArticleGoogle Scholar
- Moram MA, Barber ZH, Humphreys CJ: Accurate experimental determination of the Poisson's ratio of GaN using high-resolution x-ray diffraction. J Appl Phys 2007, 102: 023505. 10.1063/1.2749484View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.